received: 25 April 2016 accepted: 08 August 2016 Published: 30 August 2016
Functionalized chitosan electrospun nanofiber for effective removal of trace arsenate from water Ling-Li Min1,2, Lu-Bin Zhong1, Yu-Ming Zheng1, Qing Liu1,2, Zhi-Huan Yuan1 & Li-Ming Yang3 An environment-friendly iron functionalized chitosan elctrospun nanofiber (ICS-ENF) was synthesized for trace arsenate removal from water. The ICS-ENF was fabricated by electrospinning a mixture of chitosan, PEO and Fe3+ followed by crosslinking with ammonia vapor. The physicochemical properties of ICS-ENF were characterized by FESEM, TEM-EDX and XRD. The ICS-ENF was found to be highly effective for As(V) adsorption at neutral pH. The As(V) adsorption occurred rapidly and achieved equilibrium within 100 min, which was well fitted by pseudo-second-order kinetics model. The As(V) adsorption decreased with increased ionic strength, suggesting an outer-sphere complexation of As(V) on ICS-ENF. Freundlich model well described the adsorption isotherm, and the maximum adsorption capacity was up to 11.2 mg/g at pH 7.2. Coexisting anions of chloride and sulfate showed negligible influence on As(V) removal, but phosphate and silicate significantly reduced As(V) adsorption by competing for adsorption sites. FTIR and XPS analysis demonstrated –NH, –OH and C–O were responsible for As(V) uptake. ICS-ENF was easily regenerated using 0.003 M NaOH, and the removal rate remained above 98% after ten successively adsorption-desorption recycles. This study extends the potential applicability of electrospun nanofibers for water purification and provides a promising approach for As(V) removal from water. Arsenic, existing as various complex forms in the aquatic environment1,2, has been identified as one of the most harmful and toxic contaminants found in the environment3–7, because the exposure to arsenic species can lead to lung and bladder cancer, skin lesions, and even death in humans8. The sources of arsenic contamination in groundwater are both natural and anthropogenic2,8. The elevation of arsenic concentration in groundwater has been reported in many countries throughout the world, which has direct consequences to pose great threat to human health. Arsenic poisoning of groundwater was first reported in Taiwan in 19682. It is estimated that there were 19.6 million people at risk of being affected by the consumption of arsenic contaminated groundwater in China9. To minimize the health problems associated with arsenic in water, the World Health Organization (WHO) had recommended a strict permissible limit of 10 μg/L as maximum arsenic contaminant level in drinking water1. Various technologies have been developed for arsenic removal, including precipitation, membrane processes, ion exchange, and adsorption2. Adsorption has been regarded as the most promising method owing to its cost effectiveness and simplicity in operation10,11, especially when the arsenic concentration is low. Recently, biosorption has been attracted more attention because the biosorbents are eco-friendly and capable of extracting trace toxic elements from a large volume of solution1,12,13. Many biosorbents have been reported for arsenic adsorption, such as bacteria cells14, plant biomass15 and chitosan based materials16,17. Recently, the development of chitosan based adsorbents for metal ions removal has been becoming a hot topic due to its special physical and chemical properties. Chitosan is a transformed polysaccharide obtained by the deacetylation of chitin and can be easily prepared in many different physical 1
CAS Key Laboratory of Urban Pollutant Conversion, Institute of Urban Environment, Chinese Academy of Sciences, Xiamen 361021, China. 2College of Resources and Environment, University of Chinese Academy of Sciences, Beijing 100049, China. 3Department of Chemical & Biomolecular Engineering, National University of Singapore, 21 Lower Kent Ridge Road, 119077, Singapore. Correspondence and requests for materials should be addressed to Y.-M.Z. (email: [email protected]
) or L.-M.Y. (email: [email protected]
) Scientific Reports | 6:32480 | DOI: 10.1038/srep32480
Figure 1. (a) TEM image, (b) line scan, and (c) EDX elemental mappings of C, Fe, O, and N on the surface of ICS-ENF. forms such as nanoparticles, gel beads, membranes and fibers18,19. Chitosan flakes20, molybdate-impregnated chitosan beads21, chitosan-coated biosorbent8, iron coated chitosan flakes22, chitosan-immobilized sodium silicate23, TiO2-impregnated chitosan beads24 and magnetic nanoparticles impregnated chitosan beads25 have been reported for the adsorptive removal of arsenic from water. It is well known that larger specific surface area for a particular adsorbent means higher adsorption capacity, and the fabrication of chitosan porous or fibrous structure will definitely enlarge its specific surface area. This could be obtained via electrospinning, an emerging technique to prepare continuous and ultrafine nanofibers26,27. Nanofibers produced by electrospinning combines the advantages of nanomaterial (high specific surface area) and bulk material (easy separation from water), which has been recently employed as one of the most effective absorbents28,29. However, chitosan has rigid D-glucosamine repeat units with regularly arranged hydroxyl and amino groups, which leads to poor electrospinnability30. Our previous study indicated that the addition of a compatible polymer, poly(ethylene oxide) (PEO), could enhance the spinnability of chitosan and yield faultless nanofibers31. The fabricated chitosan based electrospun nanofiber (CS-ENF) has been employed for arsenic removal. The results indicated that it could be an effective arsenic absorbent at acidic condition, however, the CS-ENF showed little affinity towards As(V) with the circumstance of pH around 7.031. It has been reported that some metal-based material have been incorporated into electrospun nanofibers, which could significantly enhance the composite fibers to achieve desired functional properties28. Additionally, iron-based materials were frequently considered as adsorbent for arsenic removal from water under neutral pH32–34. Therefore, in this work, Fe3+ was selected as the additive to modify the properties of CS-ENF, and the iron functionalized chitosan based elctrospun nanofiber (ICS-ENF) was successfully fabricated in an environment-friendly way. The physicochemical properties and sorption mechanism were systematically explored using a variety of characterization tools, including FESEM, TEM-EDX, XRD, FTIR and XPS. Additionally, the arsenic removal performance of ICS-ENF was examined by both adsorption kinetics and isotherm study, and the influences of various experimental parameters, such as pH, ionic strength and competitive anions were also investigated. Finally, the regeneration and column tests were carried out to verify the potential reusability and reliability.
Results and Discussion
Characterization of nanofibers. The color of chitosan electrospun nanofiber changed from white to light yellow after the addition of FeCl3. The morphologies and fiber diameter distributions of both ICS-ENF and CS-ENF are shown in Fig. S1. The FESEM images show that the electrospun nanofibers were beadless, continuous and highly porous, which is also supported by TEM observed in Fig. 1. The fiber diameter distributions demonstrated that the average fiber diameter increased from 128 nm to 153 nm due to the incorporation of iron to chitosan matrix (Fig. S1a,b). The tensile modulus of the chitosan electrospun nanofiber didn’t change with the addition of 3 wt.% FeCl3 (Fig. S1c). However, a small decrease in the elongation was observed with the addition of FeCl3. Additionally, Fig. 1 represents corresponding elemental analysis of the nanofibers, which indicates that the relative content of nitrogen in ICS-ENF significantly increased after crosslinking by ammonia vapor (Fig. 1b). Furthermore, the EDX elemental mapping (Fig. 1c) demonstrated the fairly uniform distribution of Fe in the entire nanofibers which indicates that iron was successfully impregnated into the chitosan nanofiber.
Scientific Reports | 6:32480 | DOI: 10.1038/srep32480
www.nature.com/scientificreports/ Figure S2 illustrates the typical XRD patterns of CS-ENF and ICS-ENF. Two characteristic peaks of 2θ between 5 and 25° for CS-ENF were observed. The peak around 2θ = 7.5° was related to chitosan amorphous structure due to the presence of random amino groups (–NH2), while the peak in the 2θregion between 17 and 25° was corresponding to the biopolymer structure resulting from packing of the polymer chain and their inter-chain interactions35. Similar with CS-ENF nanofiber, ICS-ENF also contains two peaks, but it presented a higher crystallinity than that of CS-ENF in terms of the relatively sharp peak around 2θ = 10.1° (Fig. S2). Moreover, after doped with iron, the peak corresponding to 2θ = 21° was shifted from 20.5° to 22.5°. This is because the interactions between chitosan and metal ions such as Cr, Mn and Fe could affect the crystallinity via new covalent bonds between the biopolymer and the metal ions36. Although several diffraction peaks could be observed in the XRD patterns, the largely widen peaks and weak peak signals demonstrate the amorphous property of these nanofibers.
Effect of solution pH. Solution pH could affect the surface charge of adsorbent/adsobate, thus it could
play a crucial role in determining the behavior of adsorption system. Figure 2a demonstrates the influence of equilibrium solution pH (from 4.5 to 11.5) on the arsenic adsorption by ICS-ENF. Under the acid and weak basic conditions, ICS-ENF shows effective adsorption of As (more than 90% removal), and adsorption performance decreased slightly from 4.5 to 7.3. This indicates that ICS-ENF (with iron) represented better adsorption capability than that of CS-ENF (without iron), which showed little affinity towards As(V) with the circumstance of pH around 7.031. In addition, ICS-ENF has high adsorption capability at pH = 7, which is very desirable because most natural water bodies are at near neutral condition. However, with the further increasing pH value from a turning-point at 7.3, the adsorption of As(V) dramatically declines and even no adsorption process was observed upon pH up to 11.3. Similar phenomenon has been reported for the adsorption of As(V) by Zr(IV) loaded orange waste gel1 and the adsorption of As37 by Fe-Mn binary oxide38. Such behavior could be explained in terms of pHpzc of the adsorbent in the solution (pHpzc = 6.3, Fig. 2b), as As(V) adsorption would be facilitated by electrostatic interaction between negatively charged As(V) species (H2AsO4− and HAsO42− are predominant in the experimental pH range) and positively charged absorbent surface. In this case, the higher removal efficiency was due to the abundant protonation of the adsorption sites on ICS-ENF, which interacted with negatively charged arsenate species at pH